Potřebujeme váš souhlas k využití jednotlivých dat, aby se vám mimo jiné mohly ukazovat informace týkající se vašich zájmů. Souhlas udělíte kliknutím na tlačítko „OK“.
Standard Test Method for Abrasion Resistance of Horizontal Concrete SurfacesPřeložit název
NORMA vydána dne 1.10.2019
Označení normy: ASTM C779/C779M-19
Datum vydání normy: 1.10.2019
Kód zboží: NS-976091
Počet stran: 6
Přibližná hmotnost: 18 g (0.04 liber)
Země: Americká technická norma
Kategorie: Technické normy ASTM
abrasion, concrete, impact, surface treatments, wear,, ICS Number Code 91.100.30 (Concrete and concrete products)
|Significance and Use|
4.1 The three test methods provide simulated abrasion conditions, which can be used to evaluate the effects on abrasion resistance of concrete, concrete materials, and curing or finishing procedures. They may also be used for quality acceptance of products and surface exposed to wear. They are not intended to provide a quantitative measurement of length of service.
4.2 The equipment used by each of these procedures is portable and thus suitable for either laboratory or field testing. The three procedures determine the relative wear of concrete surfaces as follows:
4.2.1 Procedure A—The revolving-disk machine operates by sliding and scuffing of steel disks in conjunction with abrasive grit.
4.2.2 Procedure B—The dressing-wheel machine operates by impact and sliding friction of steel dressing wheels.
4.2.3 Procedure C—The ball-bearing machine operates by high-contact stresses, impact, and sliding friction from steel balls.
Note 2: Diagrams of three machines meeting these specifications are shown in , , and .
FIG. 1 Revolving Disks Abrasion Test Machine
FIG. 2 Dressing Wheel Abrasion Test Machine
FIG. 3 Ball Bearing Abrasion Test Machine
1.1 This test method covers three procedures for determining the relative abrasion resistance of horizontal concrete surfaces. The procedures differ in the type and degree of abrasive force they impart, and are intended for use in determining variations in surface properties of concrete affected by mixture proportions, finishing, and surface treatment. They are not intended to provide a quantitative measurement of the length of service that may be expected from a specific surface.
1.2 The values stated in either SI units or inch-pound units are to be regarded separately as standard. Within the text, the inch-pound units are shown in brackets. The values stated in each system may not be exact equivalents; therefore, each system shall be used independently of each other.
1.3 The text of this standard references notes and footnotes that provide explanatory material. These notes and footnotes (excluding those in tables and figures) shall not be considered as requirements of this standard.
1.4 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety, health, and environmental practices and determine the applicability of regulatory limitations prior to use. Note 1: Other procedures are available for measuring the abrasion resistance of concrete surfaces in addition to the three procedures contained in this test method. Consideration should be given to Test Methods and . The test method most closely representing service conditions should be used.
1.5 This international standard was developed in accordance with internationally recognized principles on standardization established in the Decision on Principles for the Development of International Standards, Guides and Recommendations issued by the World Trade Organization Technical Barriers to Trade (TBT) Committee.
|2. Referenced Documents|
Poslední aktualizace: 23.05.2022 (Počet položek: 2 568 759)
© Copyright 2022 NORMSERVIS s.r.o.